- By
**eddy** - Follow User

- 238 Views
- Uploaded on

Download Presentation
## ELASTICITY

**An Image/Link below is provided (as is) to download presentation**

Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.

- - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - -

Presentation Transcript

- Elasticity
- Elasticity of Composites
- Viscoelasticity

Elasticity: Theory, Applications and Numerics

Martin H. Sadd

Elsevier Butterworth-Heinemann, Oxford (2005)

Revise modes of deformation, stress, strain and other basics (click here) before starting this chapter etc.

What kind of mechanical behaviour phenomena does one have to understand?

- Phenomenologically mechanical behaviour can be understood as in the flow diagram below.
- Multiple mechanisms may be associated with these phenomena (e.g. creep can occur by diffusion, grain boundary sliding etc.).
- These phenomena may lead to the failure of a material.

Mechanical Behaviour

Elasticity

Recoverable deformation

Permanent deformation

Plasticity

Fracture

Propagation of cracks in a material

Fatigue

Oscillatory loading

Creep

Elongation at constant load at High temperatures

Note: above is a ‘broad’ classification for ‘convenience’. E.g. Creep is also leads to plastic deformation!

Instantaneous

Elastic

Time dependent

Anelasticity

Deformation

Instantaneous

Plastic

Time dependent

Permanent

Viscoelasticity

- Elastic deformation is reversible deformation- i.e. when load/forces/constraints are released the body returns to its original configuration (shape and size).
- Elastic deformation can be caused by tension/compression or shear forces.
- Usually in metals and ceramics elastic deformation is seen at low strains (less than ~10–3).
- The elastic behaviour of metals and ceramics is usually linear.

Linear

E.g. Al deformed at small strains

Elasticity

Non-linear

E.g. deformation of an elastomer like rubber

- Let us consider the stretching of bonds (leading to elastic deformation).
- Atoms in a solid feel an attractive force at larger atomic separations and feel a repulsive force (when electron clouds ‘overlap too much’) at shorter separations. (At very large separations there is no force felt).
- The energy and the force (which is a gradient of the energy field) display functional behaviour as below.

Energy

Force

Repulsive

Attractive

The plots of these functions is shown in the next slide

A,B,m,n → constantsm > n

Repulsive

r0

Force (F) →

Potential energy (U) →

r →

r →

r0

Attractive

Attractive

Equilibrium separation

r0

Elastic modulus is the slope of the Force-interatomic spacing curve (F-r curve), at the

Near r0 the red line (tangent to the F-r curve at r = r0)coincides with the blue line (F-r) curve

r →

Force →

r0

For displacements around r0→ Force-displacement curve is approximately linear THE LINEAR ELASTIC REGION

- Young’s modulus is :: to the –ve slope of the F-r curve at r = r0

Stress →

Tension

strain →

Compression

** Young’s modulus is not an elastic modulus but an elastic constant

Stress-strain curve for an elastomer

Tension

T due to uncoilingof polymer chains

Stress →

C

strain →

T

Due to efficient filling of space

Compression

C

T

>

- = E. E → Young’s modulus
- = G. G → Shear modulus
- hydrodynami = K.volumetric strain K → Bulk modulus

- Materials with strong bonds have a deep potential energy well with a high curvature high elastic modulus
- Along the period of a periodic table the covalent character of the bond and its strength increase systematic increase in elastic modulus
- Down a period the covalent character of the bonding ↓ ↓ in Y
- On heating the elastic modulus decrease: 0 K → M.P, 10-20% ↓ in modulus

Anisotropy in the Elastic modulus

- In a crystal the interatomic distance varies with direction → elastic anisotropy
- Elastic anisotropy is especially pronounced in materials with ► two kinds of bonds E.g. in graphite E [1010] = 950 GPa, E [0001] = 8 GPa ► Two kinds of ordering along two directions E.g. Decagonal QC E [100000] E [000001]

Elastic modulus

Property

Geometry dependence

Elastic modulus in design

- Stiffnessof a material is its ability to resist elastic deformation of deflection on loading → depends on the geometry of the component.
- High modulus in conjunction with good ductility should be chosen (good ductility avoids catastrophic failure in case of accidental overloading)
- Covalently bonded materials- e.g. diamond have high E (1140 GPa) BUT brittle
- Ionic solids are also very brittle

► First transition series → good combination of ductility & modulus (200 GPa)► Second & third transition series → even higher modulus, but higher density

- POLYMERS► Polymers can have good plasticity → but low modulus dependent on

◘ the nature of secondary bonds- Van der Walls / hydrogen◘ presence of bulky side groups◘ branching in the chains Unbranched polyethylene E = 0.2 GPa, Polystyrene with large phenyl side group E = 3 GPa, 3D network polymer phenol formaldehyde E = 3-5 GPa◘ cross-linking

Increasing the modulus of a material

- METALS

► By suitably alloying the Young’s modulus can be increased

► But E is a structure (microstructure) insensitive property the increase is fraction added► TiB2 (~ spherical, in equilibrium with matrix) added to Fe to increase E

- COMPOSITES► A second phase (reinforcement)can be added to a low E material to ↑ E(particles, fibres, laminates)► The second phase can be brittle and the ductility is provided by the matrix → if reinforcement fractures the crack is stopped by the matrix

Laminate composite

Alignedfiber composite

Particulate composite

Modulus parallel to the direction of the fiberes

- Under iso-strain conditions
- I.e. parallel configuration
- m-matrix, f-fibre, c-composite

Volume fractions

Composite modulus in isostress and isostrain conditions

Voigt averaging

- Under iso-strain conditions [m = f = c]
- I.e. ~ resistances in series configuration

- Under iso-stress conditions [m = f = c]
- I.e. ~ resistances in parallel configuration
- Usually not found in practice

Reuss averaging

Ef

Isostrain

Ec→

Isostress

For a given fiber fraction f, the modulii of various conceivable composites lie between an upper bound given by isostrain conditionand a lower bound given by isostress condition

Em

f

A

B

Volume fraction →

Download Presentation

Connecting to Server..